- 44 Views
- Uploaded on
- Presentation posted in: General

Unit 18 Persistent currents and dynamic effects

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Unit 18Persistent currentsand dynamic effects

Helene Felice, SorenPrestemon

Lawrence Berkeley National Laboratory (LBNL)

Paolo Ferracinand EzioTodesco

European Organization for Nuclear Research (CERN)

- Each conductor in a magnetic field tends to shield itself from the field – what happens for superconducting cables in a magnet ?
- Is there a dependence on ramp rate, and on the history of the magnet ?
- Are these effect large ? How can we remove them or live with them ?
- These slides heavily rely on the lecture “Dynamic effects in superconducting magnets” by A. Jain at USPAS, Phoenix 2006, and on chapter 6 of Schmuser

1. Persistent currents

2. Decay

3. Snap-back

4. Ramp effects

- Superconductor slab in external field
- A superconductor tries to shield itself from a magnetic field
- The shielding is made through currents that flow in each filament
- These currents flow inside the superconductor and therefore have no resistance (persistent)
- To maximize the shielded area, the persistent currents must have the largest possible current density, i.e. the critical current – which depends on the external field (critical state model)
- These induced currents perturb the field harmonics

- Superconductor slab in external field
- For low external fields, the critical
current flows in the outer skin to

generate a field opposite to the

external one – inside the field is zero

- When the external field rises, the
area filled with shielding currents

increases

- For low external fields, the critical

- Superconductor slab in external field
- When the external field reaches a
given value (penetration field),

all the superconductor is filled with

shielding currents

- Beyond this value, the superconductor
cannot do anything more to shield

itself and a magnetic field is present

inside it

- When the external field reaches a

- Circular filament in external field
- Hypothesis: currents flow in an elliptical
shell (Bean model)

- A bit of trigonometry gives the shielding
condition determining b

- At full penetration one has b=0 and
the magnetic field is the penetration

field

- Hypothesis: currents flow in an elliptical

- Magnetization in a circular filament in external field
- Magnetization estimate in the Bean model
- At full penetration the magnetization is

Mr. Bean, English

(born on 6 January 1955)

- Estimating penetration field
- Critical current surface vs field
use parameterization for low j

- Critical current vs penetration field
- Filament size is ~ 5-100 m
(see Unit 4)

- The penetration field is in general rather low – at high field filaments are fully penetrated

- Critical current surface vs field

- The phenomenology in a circular filament in external field ramping down
- We reached the condition of full penetration
- If now we ramp down, the external layer
of the superconductor will have opposite

current to continue the shielding

- The shielding feature depend not only on the
field but also on the previous fields:

hysteresis effect

- Hysteresis of the magnetization

From A. Jain, USPAS 2007, Dynamiceffects in superconductingmagnets, pg. 18

- Persistent currents depend on
- External parameters: magnetic field and its previous values – but not on the rate of change of the field !
- Filament parameter: size and geometry
- Superconductor parameter: critical current

- For low external fields, the critical current is larger and therefore the persistent current and induced magnetization are larger
- At large external fields the critical current becomes smaller and therefore the effect is smaller

- Magnetic field in the coil has large variations in module and direction
- Filament magnetization induces a perturbation in main field and harmonics
- For larger fields, the harmonics are further reduced by the normalization

- Measurements of the magnetization

Magnetizationmeasurement in LHC cableCourtesy of L. Bottura et al.

Magnetization measurement in HERA cable From P. Schmuser, pg. 85 Fig. 6.3

- A way to compute persistent currents
- Calculate the field map in each strand of the coil (and its previous values)
- Estimate the critical current vs field using measurements or a parameterization – note that values for low fields are very relevant
- Compute the persistent currents of the filament using a geometrical model, and scale them to the strand
- Scale the magnetization to take into account of
the transport current – it must flow somewhere !

Reduction factor is

- Evaluate the effect of these additional currents to the main field and to the field harmonics
- Several codes can do this evaluation – Roxie, …

- Comparison measurements vs model
- A good agreement is found – agreement at 90%

- Spread of persistent current given by
- Differences in the critical current
- Differences in the filament geometry, deformed after cabling

Persistent current measured vs computed in HERA dipoles and quadrupoles - From P. Schmuser, pg. 87 Fig. 6.5

Persistent current measured vs computed in Tevatron dipoles - From P. Bauer et al, FNAL TD-02-040 (2004)

- Even with the finest filaments (5 m) the persistent current give several units in allowed multipoles at injection
- How to cure this effect ? Several strategies

- Change the hardware (not cheap …)
- Of the cable: further reduce the filament size – feasible ?
- Of the machine: reduce the energy range, i.e. increase the injection current

- Design compensation: optimize coil geometry, such that harmonics are minimized at injection
- Drawback: at high field harmonics will be not optimized, but the beam is smaller …

- Active compensation through correction magnets (as in HERA, LHC)
- Passive compensation through ferromagnetic shims or ferromagnetic cold bore

1. Persistent currents

2. Decay

3. Snap-back

4. Ramp effects

- Phenomenology
- The injection of the beam is not instantaneous - takes minutes
- Tevatron: 30 minutes to 2 hours HERA: around 20 minutes
- LHC: 20 minutes

- During the injection the field is constant,
and one observes a decay of main field

and multipolar components units

- First observed in Tevatron in 1987
[R. Hanft et al., Appl. Supercond. Conf. (1988), also in TM-1542]

- First observed in Tevatron in 1987
- Equations proposed to fit the decay
- Logarithmic decay (HERA, Tevatron)
- Double exponential (RHIC, LHC)

- The injection of the beam is not instantaneous - takes minutes

Decay of b3 in HERA dipoles versus time, from Schmuser pg. 90, fig 6.8

- Origins
- Thermally activated flux creep inducing a decrease in the critical current density
- It is temperature dependent
- Produces a logarithmic decay

- Boundary induced coupling currents
- The strands carry different currents
- Current redistribution can affect the magnetization due to the changes in the local field

- There are indications that both mechanisms are involved in the decay of magnetization

- Thermally activated flux creep inducing a decrease in the critical current density

- Dependence on the previous history
- The amplitude of the decay depends on the parameters of the previous cycles
- Proportional to the flat-top current of the previous cycle
- Decreases for longer back-porch
- Saturates for flat-top duration longer than 1 h

- The amplitude of the decay depends on the parameters of the previous cycles

The cycle used for powering Tevatron dipoles, from P. Bauer et al, FNAL TD-02-040 (2004)

1. Persistent currents

2. Decay

3. Snap-back

4. Ramp effects

- Phenomenology
- At the end of the injection, the beam is accelerated and the field is ramped up
- In that moment, the decay of persistent currents disappears and the previous values are recovered

Snapback phenomenology in RHIC dipoles, from A. Jain, USPAS 2006, « Dynamic effects and … », slide 27

- Snapback versus current
- The snapback versus current (i.e. versus field, and versus time) dependence is exponential
- The snapback takes place in a few seconds – very fast phenomena

Snapback in b3 versus time, LHC main dipoles, from L. Bottura et al, IEEE Trans. Appl. Supercond. 15 (2005) 1217-20.

- Snapback versus current
- Two parameters: amplitude (the same of the decay) and “time” constant I
- Measurements show that they are proportional
- The constant depends on the magnet design
- One can justify this proportionality through a model

- Two parameters: amplitude (the same of the decay) and “time” constant I

Linear relation between snapback constants for Tevatron (right) and LHC (left) dipoles from L. Bottura et al, IEEE Trans. Appl. Supercond. 15 (2005) 1217-20.

1. Persistent currents

2. Decay

3. Snap-back

4. Ramp effects

- The ramping of the magnet induces a variation of the flux with time in loops made by strands
- This variable flux can induce currents which are
- Proportional to the ramp rate
- Proportional to the area of the loop
- Inversely proportional to the inter-strand cross-contact resistance

- These currents may perturb the field homogeneity for high ramp rates
- A cure: increase the inter-strand resistance by special coating
- For example, in the LHC dipoles the ramp rate is 10 A/s, the inter-strand resistance is > 15-40 , and the impact on field quality is negligible

- This variable flux can induce currents which are
- Another effect can come from flux variation in loops made by filaments
- Usually called coupling currents

- Persistent currents
- The mechanism
- The conductor shields itself from the external magnetic field this generates shielding currents inside the conductor field perturbation

- Features
- Contribution is very relevant at injection, disappears at high field
- Contribution on allowed harmonics, proportional to filament size, gets worse with large energy sweep
- Contribution depends on the previous values of the magnetic field, but not on the rate of magnetic field change (hysteretic phenomena)

- Reliable models can predict the persistent currents
- Corrections
- Passive correction with ferromagnetic shims
- Smaller filament, smaller energy sweep
- Active correction with corrector magnets

- The mechanism

- Decay
- The mechanism
- When the field is constant (this happens at injection energy) the magnetization decays with time due to different mechanisms
- Flux creep
- Boundary induced coupling currents

- When the field is constant (this happens at injection energy) the magnetization decays with time due to different mechanisms
- Features
- Scale time is 100 s
- Semi-empirical fits with exponential or logarithms are used
- Contribution depends on the previous history, including the rate of magnetic field change (dynamic effect)

- No quantitative predictions available
- Corrections
- Phenomena are slow, corrector magnets are used to compensate on the fly

- The mechanism

- Snapback
- The mechanism
- When the field is ramped up again, all the decay of persistent currents is wiped out and the previous state is recovered

- Features
- Scale time is 1 s
- Fit with exponential, based on heuristic model, are used
- The amplitude of the snapback and the time constant are proportional – can be justified with an heuristic model

- Corrections
- Phenomena are fast, they cannot be corrected on the fly but correction curves should be implemented based on measurements

- The mechanism

- We now finished the outline of the phenomena involved in the determination of the field homogeneity in a superconducting magnet
- Geometry of cables
- Iron effect
- Deformations
- Hysteresis
- Time dependent effect

- In the next unit we will discuss
- agreement between the field model and the measurements,
- agreement between field measurements and expected effects measured on the beam

- General
- M. N. Wilson, Ch. ?
- Schmuser, Ch. 6 and 7
- L. Bottura, “Field dynamics in superconducting magnets for particle accelerators”, CERN 98-05 (1998).
- Classes given by A. Jain at USPAS 2006, Unit 7
- Ph. D. thesis of A. Verweij

- Decay and snap-back
- L. Bottura et al, IEEE Trans. Appl. Supercond. 15 (2005) 1217-20
- N. Sammut Ph. D. thesis on the LHC magnets
- Several works by P. Bauer et al carried out in 2000-2005 at FNAL on Tevatron
- Complete references on the works on Hera can be found in Schuser book

- L. Bottura and A. Jain for discussions, comments and useful advices